advertisement

The Diffusion Equation — I 3.205 L2 10/31/06 1 Fick’s Laws of Diffusion • Fick’s first law r J = "D#c ! • The diffusivity, D, is a second-rank tensor Fick’s second law r "c = #$ % J "t ! 3.205 L2 10/31/06 2 Self-diffusion • Self-diffusion in a chemically pure material Involves diffusion of a radiotracer isotope that, while chemically identical to the host element, is easily tracked. C J*1 3.205 L2 10/31/06 # L11 L1*1 & *c*1 *c*1 = "kT % " = " *D ) () *x $ c1 c*1 ' *x 3 Self-diffusion, cont’d • Self-diffusion in a homogeneous binary solution Involves diffusion of a radiotracer isotope solute species that is easily tracked. C J*1 3.205 L2 10/31/06 ! # L11 L1*1 & *c*1 *c*1 = "kT % " ) = " *D ) ( 1 *x $ c1 c*1 ' *x 4 Vacancy mechanism of diffusion • Self-diffusion in crystals, and diffusion of species in substitutional alloys, generally occurs by the vacancy mechanism. Figure removed due to copyright restrictions. See Figure 8.2 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter. Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891. • Interdiffusion in an alloy with gradients of c # L11 L12 &# )ln *1 )ln + & )c1 )c1 = "kT % " + = "D1 , (%1+ (, )x $ c1 c2 '$ )ln c1 )ln c1 ' )x % #ln $1 ( and D1 " '1+ * +*D1 is the intrinsic diffusivity & #ln c1 ) 3.205 L2 10/31/06 J1C ! 5 Interdiffusion • In a substitutional alloy of species 1 and 2, the self diffusivities D1 and D2 are generally different. Figure removed due to copyright restrictions. See Figure 3.3 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter. Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891. For the case illustrated, D1 > D2 and the species move at different rates. The flux difference is balanced by a net flow of vacancies from right to left. 3.205 L2 10/31/06 6 The Kirkendall effect • • • Net flux of vacancies to the left makes inter diffusion zone migrate toward the left in the figure. Inert particles placed at the interface of the diffusion couple move toward the left. Vacancies must be created on the right and migrate to the left of the interdiffusion zone where they are destroyed. Creation/destruction of vacancies is accomplished by dislocation climb. 3.205 L2 10/31/06 7 Description of interdiffusion • Interdiffusion is usually described in a volumefixed reference frame, often called the laboratory frame, fixed relative to the specimen ends. In this frame, %c %c J1V = "[c1#1D2 + c2#2 D1 ] $ 1 = D˜ $ 1 %x %x %c %c J 2V = "[c1#1D2 + c2#2 D1 ] $ 2 = D˜ $ 2 %x %x and D˜ = c1"1D2 + c2"2 D1 ! ! 3.205 L2 10/31/06 is known as the interdiffusivity 8 Other driving forces for diffusion • • • • • We discussed above diffusion driven by gradients of chemical potential…more complex phenomena include: Diffusion of charged ions in ionic conductors Electromigration in metals Diffusion in a thermal gradient Capillarity-driven diffusion Stress-driven diffusion 3.205 L2 10/31/06 9 Capillarity-driven diffusion • Occurs as a result of the Gibbs-Thomson effect, which relates to the way chemical potentials differ in systems with curved interfaces, relative to systems with planar interfaces. Figure removed due to copyright restrictions. See Figure 3.7 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter. Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891. 3.205 L2 10/31/06 10 Stress-driven diffusion • Interstitials in a crystal are point centers of dilation and have associated stress fields that can interact strongly with other sources of inhomogeneous stress, e.g. dislocations. Figures removed due to copyright restrictions. See Figures 3.8 and 3.9 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter. Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891. 3.205 L2 10/31/06 11 Stress-driven diffusion, cont’d • The diffusion potential Φ for an interstitial component 1 has an additional term proportional to the local hydrostatic stress P "1 = µ1 + #1P and the diffusion equation takes the form ( % c1$1 ! J1 = "L11#(µ1 + $1P) = "D1'#c1 + #P * & ) kT 3.205 L2 10/31/06 ! 12